Presentation on theme: "Timber Mr Noor M S Hasan. Introduction Timber is by no means outdated and continues to play a major part in general building, particularly in domestic."— Presentation transcript:
Timber Mr Noor M S Hasan
Introduction Timber is by no means outdated and continues to play a major part in general building, particularly in domestic dwellings and furniture. More recently, use in larger public, commercial and industrial buildings in the form of timber frames, trussed rafters and glued laminated sections has increased.
Attractive properties of timber and timber products: They are natural products, hence they are a renewable resource. With properly managed forestry policies trees can be effective in reducing the carbon dioxide levels in the atmosphere, thereby reducing global warming. Manufacturing of timber products require much less energy than alternative materials. Energy required in confined to felling, conversion, machining and transport.
Continued……. The material does not pose any disposal problem after use. It rots naturally, reverting to carbon dioxide enabling the growth cycle to be repeated. Timber has a high strength to weight ratio and for this reason is particularly useful for roofing where superimposed loads are limited. Timber is of aesthetically pleasing appearance. Timber has a low thermal conductivity, hence it has a warm ‘feel’.
Continued……… The material is easily worked with hand tools and joined with nails or screws. Strong joints can be formed with adhesives. Modern adhesives penetrate the wood and many are both strong and waterproof once set. Structural timber sections have good fire resistance.
Problems associated with the use of timber are: The material may be very variable due to the effects of ‘imperfections’ such as knots, grain, and defects such as ‘shakes’ Timber is subject to movement and possible distortion when its moisture content changes. Timber is subject to fungal and insect attack. Untreated timber burns readily in fire and therefore continues a fire hazard, contributing to the fuel load of the building and spreading the fire by flame. Timber is subject to creep under load, especially its moisture content is subject to change.
Structure of Wood: Wood is naturally occurring fibrous composite. Fibres consisting chiefly of crystalline cellulose. Timber being a very important means of reducing atmospheric carbon dioxide. As long as the timber is preserved it helps to reduce atmospheric carbon dioxide. But if the timber is ultimately burned or allowed to rot, it reverts to atmospheric carbon dioxide and the benefit is lost.
Classification of Timber Softwood: Figure 1: Radial, tangential and transverse sections
Figure 1 shows a cut portion of a 5-year old softwood log. Longitudinal – the direction of growth of the tree. Radial – running outwards towards the bark. Tangential – running around the perimeter of the tree. It is evident that cells run chiefly in two directions- longitudinally and radially. Most cells run in the longitudinal direction in order to support the tree and to provide food and conduction.
Further food conduction and storage are provided by rays which run in the radial direction. Rays also increase the strength of the timber in this direction. In softwoods the function of both food conduction and support are mainly fulfilled by a type of cell known as a tracheid. Additionally, in the rays there are hollow food storage cells known as parenchyma. Figure 2 (a) shows a simplified radial section of the softwood cell structure. Adjacent cells are joined in all directions by pits which are responsible for the transmission of food between them. The rays in softwood are usually small and not visible to the naked eye.
Figure 3 shows a scanning electron microscope photograph of cut transverse, radial and tangential surfaces of a sample of European redwood (Pinus sylvestris)
Softwood timbers are coniferous (cone bearing) and have a needle or fern-like foliage which is retained in winter. They grow relatively quickly, the resultant wood generally being soft, of low density and easily worked. Softwoods are substantially more economical than hardwood though they are in general less durable. They are now the most widely used types of wood for general structural purposes. Commonly used species are Scots pine (redwood), European spruce (whitewood), Douglas fir and cedar.
It should be noted that wood contains natural resins which make it unattractive to fungi and insects which gives very good durability. Hardwoods: Hardwood have a more complex cell structure than softwoods, structural support being provided by long, thick-walled cells known as fibres, while food conduction is by means of thin-walled tubular cells called vessels (Figure 2 (b)). Parenchyma (food storage cells) are again present both as longitudinal strands and in rays. Cells are again interconnected by pits.
Hardwoods can be subdivided into ring- porous varieties, in which the vessels are mainly concentrated in springwood, and diffuse-porous woods, in which there is a more even distribution of vessels. Figure 4 shows a scanning electron microscope photograph of Oak- a typical ring porous wood. And it is also noticeable the prominence of the rays in the wood.
Figure 4: Scanning electron microscope photograph of Oak (Quercus robus), a ring porous hardwood.
Hardwoods generally grow more easily than softwoods and are usually harder, denser, stronger and more durable. These are, however, exceptions such as balsa and poplar- fast-growing hardwoods with poor structural properties and durability. Hardwoods may be used where their durability is beneficial- for example, in window and door sills; or in high quality joinery. They are also extensively used in producing veneers for doors and furniture.
Heartwood and Sapwood: The food conduction and storage functions of trees are fulfilled by the outer, more newly grown layers of cells, referred to as sapwood, the inner layers being referred to as heartwood. Heartwood is normally darker in colour than sapwood and, on account of its acidity, tends to be more resistant to fungi and insects in service. In young trees most of the wood is sapwood, while in old trees as much as 80 percent of the wood is heartwood.
Continued……… Bearing in mind the difference in durability of the two types, it will be evident that older trees tend to give timber of a better quality. Traditionally sapwood was often rejected, but since this would be uneconomic when, as is now common, young trees are employed, other means of ensuring durability may be advisable such as the use of preservatives.
Effects of Moisture in Timber: The moisture content of timber is defined as: Moisture content = (mass of water present in a sample / mass of the sample when oven dry)* 100 If the mass of water contained exceeds the mass of dry timber, a moisture content of over 100 percent is obtained and this is not unusual in newly felled (green) timber. The sapwood tends to contain more moisture at the same time of felling, the average moisture content being about 130 percent, though values of over 200 percent are possible.
In heartwood the moisture content is more likely to be around 50 percent. The moisture content of green timber varies considerably with species. Denser timbers, most hardwoods, have smaller cavities and larger cell walls, hence they can store less water. The moisture content of timber is service is greatly influenced by the fact that wood is hygroscopic, that is, it tends to attract water from a damp atmosphere and give up water to a dry atmosphere.
In consequence timber will adopt an equilibrium moisture content in a given environment, depending on the relative humidity of that environment. Since increase of temperature tends to reduce relative humidity, it also results in reduced equilibrium moisture contents. At moisture contents in excess of 20 percent, timber becomes susceptible to fungal attack, hence the importance of providing a dry environment will be appreciated.
Recent surveys have shown that timber in service often has a lower moisture content than was formerly assumed in design. Major factors in this are central heating and air conditioning. In winter cold air is admitted by means of ventilation and this can only contain limited quantities of water. On heating, the relative humidity drops to quit a low value, the moisture content of timber falling in consequence.
In very warm buildings such as hospitals the moisture content may drop to as low as 8 percent. In normally ventilated buildings which are centrally heated, moisture contents tend to fall towards the end of the winter period. In summer, air-conditioning systems may similarly reduce moisture contents of timber since they condense water out during the cooling cycle.
Seasoning: Seasoning is the controlled reduction of the moisture content of timber to a level appropriate to its end use. Correctly seasoned timber should not be subject to further significant movement once in service, unless, of course, leaks occur. Seasoned timber is also immune to fungal attack, is stronger, has lower density and is therefore easier to handle or transport; it is also easier to work, glue, paint or preserve than wet timber.
Air Seasoning: Traditionally a large amount of timber was air seasoned by stacking in open formations in a roofed enclosure. Drying takes place due to the effects of wind and sun, in a time which depends on the type and section size of timbers, the size of air gaps between them and the climatic conditions. The process minimises damage but is slow, often taking several years to complete, and will not reduce the moisture content below about 16 percent.
Kiln Seasoning: This type of seasoning involves heating the timber in sealed chambers, initially using steam to maintain saturation, the humidity then being progressively reduced to produce drying. Water has a lower surface tension and viscosity at higher temperatures and therefore flows more freely through the timber so that drying can take place more rapidly without damage. Drying schedules depend on the type and size of timber sections and their initial and target moisture content.
Kiln seasoning takes about one week per 25 mm thickness for softwoods and about two weeks per 25 mm thickness for hardwoods. The process has the advantage that it sterilises the wood and can reduce moisture contents to lower levels than air seasoning- values of about 12 percent can be reached quit easily.
Factors affecting the Distortion of Timber prior to use: Species of timber: Some timbers that have similar moisture movements in the radial and tangential directions- for example, Douglas fir and utile- are inherently less prone to distortion than timbers that have high relative movements- for example, European redwood and beech. Method of conversion: Quarter sawn timber distorts less on moisture change than flat sawn timber, though the latter has a more interesting grain pattern. Pieces of timber which contain the pith are also more prone to distortion, especially springing. Where the piece is not cut parallel to the longitudinal axis, bowing, springing and twisting are likely.
Continued…….. Slope of grain: Twisting is often caused when the grain is not straight or when the density of the wood varies- for example, due to unequal growth on different sides of the tree. Timber having uniform and straight grain is less likely to undergo distortion. Stacking procedure: Each piece of timber in a stack must be adequately supported by ‘stickers’ prior to and during seasoning in order to avoid distortion due to self- weight. Twisting of timber can be largely avoided if it is held firmly in stacks during seasoning. Moisture changes prior to installation: Rapid moisture changes after seasoning – for example, wetting or severe drying on occupation of new properties- can lead to serious distortion. Such changes should be avoided.
Figure 5: Types of distortion in timber and their measurement
Durability of Timber: Timber has remarkably good resistance to deterioration by atmospheric exposure. It is virtually unaffected by agencies such as rain, frost and acids, which are responsible for damage to other types of materials. The action of sunlight is only slight, prolonged exposure degrading the lignin adhesive so that the timber surface is bleached, becoming slightly fibrous. The main mechanisms of attack involve its being used – by plants in the form of fungi and by insects.
Fungal attack: Growth of all fungi in timber requires a moisture contents of at least 20 per cent. The enzyme action necessary for fungal growth can not take place in completely dry timber. There are numerous varieties, some attacking the growing tree or the unseasoned green timber, while others are able to attack the wood in service. Where the cellulose only is destroyed, the wood breaks into small cubes and the rot is known as brown rot.
Where both cellulose and lignin are destroyed, the wood becomes soft and fibrous, the rot being known as white rot. Dry Rot: Dry rot (Serpula lacrymans, formerly called Merulius lacrymans) is a brown rot, so named because it finally leaves the wood in a dry, friable condition. The greatest risk is in areas without satisfactory ventilation such as cavities in floors or walls, especially where there are leaks or rising damp.
Dry rot can be serious problem once established, since it is often very difficult to eradicate the hyphae completely, especially in brickwork or plaster or where access is limited. Normal remedial measures are: Cut out and burn all visibly affected timber, together with an extra 600mm of apparently sound neighbouring timber which may contain hyphae. Remove any affected plaster, again working beyond the visibly affected area. Preserve sound exposed timber and treat surrounding brick or concrete with a fungicide.
Replace affected timber with preserved, seasoned timber. Use Zinc Oxychloride in paint or plaster coatings applied to affected wall surfaces. And this has a fungicidal action. Rectify the cause of dampness. Wet Rot: Wet rots require higher moisture contents in order to thrive, optimum values being in the region of 50 per cent. There are many types of wet rot such as Coniophora puteana and Phellinus contiguus.
Coniophora puteana (‘cellular fungus’) is commonly found in very damp situations in buildings – especially basements or cellars. The fungus is of the brown variety and leads to cube formation, especially in large timber sections, though a skin of sound timber may be present. Surface undulations in timber may be the first signs of damage. Affected wood turns dark brown or black but fruiting bodies are rare.
Phellinus contiguus is responsible for a considerable increase in window joinery decay which has occurred over the last 20 years or so. It is a white rot, hence wood breaks into soft strands. The cause of the increase in this type of rot is probably the use of sapwood in joinery, which, together with poor design and inadequate glues, leads to water penetration at joint. Since most journey of this type is painted, the first signs of attack are often undulations in or splitting of the paint film.
Insect Attack: Insects such as beetles that commonly infest timber in construction, have a characteristic life cycle: egg, caterpillar (larva), chrysalis and finally adult beetle. Beetles then emerge from the timber and fly to new timber to lay eggs and repeat the cycle, which may take several years. Most damage is done by larvae, which burrow through the wood leaving the powder (‘frass’) behind. Flight holes are the normal visual means of locating infestations but quite advanced deterioration accompanied by serious strength loss may occur with only a small number of holes.
Dust is often ejected from these holes and an indication of the degree of current activity can be judged from the colour of exit holes and dust produced – a lighter indicates a recent attack. Insect does not require wet timber, though higher moisture content are preferred and timber under the influence of central heating is unlikely to be attacked. And it is noticeable that sapwood is much more susceptible to insect attack than heartwood. Attack is also less likely in wood products, such as chipboard, containing synthetic adhesives.
Preservatives treatment for timber (BS 1282): Preservatives should be toxic to fungi and/ or insects as required, be of sufficient chemically stability for their operational environment, be able to penetrate timber and be non-aggressive to surrounding materials. Preservatives can be classified according to type: Tar oil preservatives (BS 144): Creosotes, the best known examples, are derivations of wood or coal, though coal distillates are superior. They are only suitable for external use, since they give rise to a noticeable colour and smell.
They are however, cheap and can be applied to timber with a fairly high moisture content. They tend to creep into porous adjacent materials such as cement renderings and plaster. Water –borne preservatives (BS 4072): These consist of salts based on metals such as sodium, magnesium, zinc, copper, arsenic and boron. Copper-chrome-arsenic (CCA) is a common example. They are tolerant of some moisture in the timber, are colourless, non-flammable and non-creeping which may be painted or drying out.
Although water-based preservatives are fairly cheap, they have the disadvantage that they swell the timber and will cause corrosion of metals in contact until drying out is complete which takes about 7 days depending on timber type and section thickness. Hence they are best used as a preliminary protection followed by kiln drying, rather than as an in-situ treatment. Timber should be below fibre saturation point (28 per cent moisture content) before the application of water-based preservatives.
Organic solvent preservatives (BS 5707): Examples are chloronaphthalenes, metallic naphthanates and penta chlorophenol. Penetration is excellent provided the timber is quite dry, hence they are often preferred where only brush or spray applications are feasible. They are non-creeping, non-staining, non- corrosive to metals, non-swelling and quick drying. Painting is usually possible once drying is complete, which usually takes a few days.
Boron diffusion: In this process freshly felled timber is dipped into a concentrated borate solution which diffuses throughout the wood by means of its own moisture, hence the need to treat the wood in a ‘green’ state. The process can be used to advantage on ‘difficult’ timbers those which do not readily admit preservatives.
Application methods: The technique of application is just as important as the choice of a suitable preservative, since, of it is poorly applied, it will fail to penetrate timber sections sufficiently. The following techniques can be adopted: Brushing or spraying: These gives only limited penetration of timber, although they may be the only feasible methods for in-situ remedial work. However, if several coats are applied and the treatment is repeated periodically, a useful degree of protection is achieved.
Dipping: This involves immersing the timber in the preservative for a period, which, if long enough, can gives considerable penetration of preservative. In the ‘open tank’ method if dipping, the preservative is heated, then cooled, while the timber is submerged; this gives even better results. It is nevertheless not suited to hardwoods or low permeability softwoods.
Double-vacuum process: A vacuum is applied to timber in a sealed chamber and the preservative then introduced. The vacuum is released, forcing the preservative into the wood. After a soaking period, the vacuum is reapplied to eject excessive preservative. This process is now widely used in conjunction with organic preservatives for external joinery such as window frames.
Pressure impregnation: This is often used for injection of water-based and tar oil-based preservatives. In the empty cell process, the air surrounding the timber is compressed, the preservative introduced and then a still higher pressure applied, forcing preservative into the wood. On releasing the pressure, excess preservative is rejected. This method is more expensive in terms of the quality used and, since saturated, will take longer to dry. Good protection is nevertheless achieved.
Timber products: Most timber products are the direct consequence of the excellent bonding properties of the material. Smooth flat surfaces are easily obtained by planning and present a porous surface into which adhesives can penetrate. The adhesive therefore grips the wood, providing bond strengths that are often in excess of the cohesive strength of the material.
Timber products may offer the following advantages over solid timber: They are competitive in price on account of lower wastage rates. Smaller sections of the tree, together with defective prices and off-cuts which are not suitable for solid timber, are often perfectly acceptable for timber products. Products can be produced in much larger sizes than could be obtained in solid timber – for example, sheets or long lengths. Defects associated with solid timber can be removed or made less significant. Weakness or distortion associated with grain can be at least partly overcome.
Areas in which timber products could cause problem are: The products can only be as good as the adhesive used in its production. Some products deteriorate quickly in damp conditions – as might prevail on a building site during construction, or in areas such as kitchens or bathrooms. Some adhesives increase wear and tear on cutting tools used for processing products. Some timber products are not as aesthetically attractive as their solid timber counterparts. Bending strengths are not in general as good as those of solid timber parallel to the grain Creep levels may be increased.
Wood fibre boards: These are produced by breaking wood down into its fibres and then pressing them together. The product obtained depends on the process used (wet or dry), the adhesive used (if any) and the pressure applied. They all have smooth surfaces reflecting their fibrous nature. Some common fibre boards are: Hardboards Medium boards Softboards MDF boards Particle boards (Chip boards) Oriented strand board Ply woods Glued laminated timber (glulam)
Environmental considerations in the use of timber: This chapter began with a description of the environmental advantages of timber, including its low energy input and the fact that a growing tree is a means of controlling or even reducing levels of carbon dioxide in the atmosphere. There have nevertheless been criticisms that the construction industry is at times indiscriminate in its use of timber, some hardwoods in particular being derived from mass de- forestation projects which may, in addition to carbon dioxide implications, lead to: Land instability Soil erosion Climatic changes on a local or wider scale Disturbance of wildlife balance
Recycling timber Reuse: Demolition sites can be a useful source of quality timber. Most demolition work is in older buildings and it is found that timber that has already been in service for a century or more can be of very sound quality. In fact, such timber may well be heartwood of mature trees and perform better than modern softwood equivalents which often contain sapwood. Such timber should, of course, be checked for insect or fungal damage.
Reuse continued…… Good candidates for reuse are floorboards and parquet flooring. These are often of high quality and can be used with minimal preparation if used upside down. The reuse opportunities for timber for structural purposes are limited unless it is subjected to stress grading, and this is in general not feasible. Reuse applications are currently therefore of limited scale and operated on a local largely unstructured basis.
Recycle: Recycling wood seem to be a very attractive option for timber construction waste. However, to maintain quality and a ‘new’ appearance, particle board manufactures tend to have stringent specifications for wood chip waste. Recycled wood chip contents are currently limited to around 5 percent, so low that there is a need for a lower grade board for nominal applications which could accept larger quantities of waste material. It will be appreciated that some contaminants such as paint, adhesives and nails can be quite difficult to remove from wood. A further possibility for low grade material is to form it into insulants made from low grade wood chips and hydrated lime, being used as an in-situ insultant in the walls and floors of a timber- framed dwelling.
Recovery: This constitutes the least preferred option in that the timber is used only as a fuel. Nevertheless, it must be considered preferable to use the timber to assist in, for example, district heating schemes from combustion of waste materials, rather than simply burning the material in the open. Large bonfires are a common site on demolition sites and must be regarded as lost environmental opportunities. There have been examples of processes in which timber is pelletised for burning in special wood-burning stoves.
References TAYLOR, G.D, 2000, Materials in Construction, An Introduction, 3 rd Ed. Pearson